Thorium

90

actinium ← thorium → protactinium


Ce
↑
Th
↓
(Uqn)




periodic table




General


Name, Symbol, Number

thorium, Th, 90


Chemical series
Actinides


Group, Period, Block

n/a, 7, f


Appearance
silvery white 



Atomic mass
232.03806(2) g/mol


Electron configuration
[Rn] 6d2 7s2


Electrons per shell
2, 8, 18, 32, 18, 10, 2


Physical properties


Phase
solid


Density (near r.t.)
11.7 g/cm³


Melting point
2115 K
(1842 °C, 3348 °F)


Boiling point
5061 K
(4788 °C, 8650 °F)


Heat of fusion
13.81 kJ/mol


Heat of vaporization
514 kJ/mol


Heat capacity
(25 °C) 26.230 J/(mol·K)




Vapor pressure


P/Pa
1
10
100
1 k
10 k
100 k


at T/K
2633
2907
3248
3683
4259
5055



Atomic properties


Crystal structure
cubic face centered


Oxidation states
4
(weakly basic oxide)


Electronegativity
1.3 (Pauling scale)


Ionization energies
(more)

1st: 587 kJ/mol


2nd: 1110 kJ/mol


3rd: 1930 kJ/mol


Atomic radius
180 pm


Miscellaneous


Magnetic ordering
no data


Electrical resistivity
(0 °C) 147 nΩ·m


Thermal conductivity
(300 K) 54.0 W/(m·K)


Thermal expansion
(25 °C) 11.0 µm/(m·K)


Speed of sound (thin rod)
(20 °C) 2490 m/s


Speed of sound (thin rod)
(r.t.) 79 m/s


Shear modulus
31 GPa


Bulk modulus
54 GPa


Poisson ratio
0.27


Mohs hardness
3.0


Vickers hardness
350 MPa


Brinell hardness
400 MPa


CAS registry number
7440-29-1


Notable isotopes




Main article: Isotopes of thorium


iso

NA

half-life

DM

DE (MeV)

DP


228Th

syn

1.9116 years

α

5.520

224Ra


229Th

syn

7340 years

α

5.168

225Ra


230Th

syn

75380 years

α

4.770

226Ra


231Th

trace

25.5 hours

β

0.39

231Pa


232Th

100%

1.405×1010 years

α

4.083

228Ra


234Th

trace

24.1 days

β

0.27

234Pa


Thorium (chemical symbol Th, atomic number 90) is a naturally occurring, slightly radioactive metal and is a member of the actinide series. It can be used in magnesium alloys to impart strength, heat-resistant ceramics, gas tungsten arc welding electrodes, and in coating tungsten wire for electronic equipment. It is a fertile material for producing nuclear fuel, and is under consideration as an alternative nuclear fuel, in place of uranium. In addition, thorium dioxide may be used as a catalyst for various chemical reactions, in mantles for portable gas lights, and in high-quality glass lenses for cameras and scientific instruments.

Contents

1 Occurrence
2 History
3 Notable characteristics

3.1 Isotopes


4 Applications

4.1 Applications of thorium dioxide (ThO2)
4.2 Thorium as a nuclear fuel


5 Precautions
6 See also
7 Footnotes
8 References
9 External links
10 Credits



Occurrence
 Monazite, a rare-earth-and-thorium-phosphate mineral, is the primary source of the world's thorium.
Thorium is found in small amounts in most rocks and soils, where it is about three times more abundant than uranium, and is about as common as lead. Soil commonly contains an average of around 12 parts per million (ppm) of thorium. Thorium occurs in several minerals, the most common being the rare earth-thorium-phosphate mineral, monazite, which contains up to about 12 percent thorium oxide. There are substantial deposits in several countries. 232Th decays very slowly (its half-life is about three times the age of the earth) but other thorium isotopes occur in the thorium and uranium decay chains. Most of these are short-lived and hence much more radioactive than 232Th, though on a mass basis they are negligible. India is believed to have 25 percent of the world's thorium reserves.[1]
Current estimates (in tons) of thorium mineral reserves are as follows.[2]

380,000 Turkey
300,000 Australia
290,000 India
170,000 Norway
160,000 United States
100,000 Canada
35,000 South Africa
16,000 Brazil
95,000 Others
History
Thorium was discovered in 1828 by the Swedish chemist Jöns Jakob Berzelius, who named it after Thor, the Norse god of thunder. The metal had virtually no uses until the invention of the lantern mantle in 1885.
The crystal bar process to produce high-purity metallic thorium (or Iodide process) was discovered by Anton Eduard van Arkel and Jan Hendrik de Boer in 1925.[3]
The name ionium was given early in the study of radioactive elements to the 230Th isotope produced in the decay chain of 238U before it was realized that ionium and thorium were chemically identical. The symbol Io was used for this supposed element.

Notable characteristics
Thorium is an inner transition metal in the actinide series. It follows actinium in period seven of the periodic table.
When pure, thorium is a silvery white metal that retains its luster for several months. However, when it is contaminated with the oxide, thorium slowly tarnishes in air, becoming gray and eventually black. Thorium dioxide (ThO2), also called thoria, has one of the highest melting points of all oxides (3300°C). When heated in air, thorium metal turnings ignite and burn brilliantly with a white light.

Isotopes
Naturally occurring thorium is composed of one radioactive isotope: 232Th, which has a half-life of 14.05 billion years. Many other radioisotopes have been characterized, including 230Th, with a half-life of 75,380 years; 229Th, with a half-life of 7,340 years; and 228Th, with a half-life of 1.92 years. All the remaining radioactive isotopes have half-lives that are less than 30 days, and the majority of these have half-lives that are less than ten minutes. This element also has one meta state.
The known isotopes of thorium range in atomic weight from 209 amu (209Th)[4] to 238 amu (238Th).

Applications
Thorium is used as an alloying element in magnesium alloys, imparting high strength and creep resistance at elevated temperatures.
It is used to coat tungsten wire for electronic equipment, improving the electron emission of heated cathodes.
It has been used in gas tungsten arc welding electrodes and heat-resistant ceramics.
Uranium-thorium age dating has been used to date hominid fossils.
It is a fertile material for producing nuclear fuel. In particular, the proposed energy amplifier reactor design would employ thorium. Since thorium is more abundant than uranium, some designs of nuclear reactor incorporate thorium in their nuclear fuel cycle.
Thorium is a very effective radiation shield, although it has not been used for this purpose as much as have lead or depleted uranium.
Thorium may be used in subcritical reactors instead of uranium as fuel. This produces less waste and cannot melt down.
Applications of thorium dioxide (ThO2)
It has been used for mantles in portable gas lights. These mantles glow with a dazzling light (unrelated to radioactivity) when heated in a gas flame.
Used to control the grain size of tungsten used for electric lamps.
Used for high-temperature laboratory crucibles.
Added to glass, it helps create glasses of a high refractive index and with low dispersion. Consequently, they find application in high-quality lenses for cameras and scientific instruments.
It has been used as a catalyst:
In the conversion of ammonia to nitric acid.
In petroleum cracking.
In producing sulfuric acid.
Thorium dioxide was the active ingredient of Thorotrast, which was used as part of X-ray diagnostics. This use has been abandoned due to the carcinogenic nature of Thorotrast.
Thorium as a nuclear fuel
Thorium, as well as uranium and plutonium, can be used as fuel in a nuclear reactor. Although not fissile itself, 232Th will absorb slow neutrons to produce uranium-233 (233U), which is fissile. Hence, like 238U, it is fertile.
In one significant respect, 233U is better than the other two fissile isotopes used for nuclear fuel, 235U and plutonium-239 (239Pu), because of its higher neutron yield per neutron absorbed. Given a start with some other fissile material (235U or 239Pu), a breeding cycle similar to, but more efficient than that currently possible with the 238U-to-239Pu cycle (in slow-neutron reactors), can be set up. The 232Th absorbs a neutron to become 233Th which normally decays to protactinium-233 (233Pa) and then 233U. The irradiated fuel can then be unloaded from the reactor, the 233U separated from the thorium (a relatively simple process since it involves chemical instead of isotopic separation), and fed back into another reactor as part of a closed nuclear fuel cycle.
There are, however, several problems with the use of thorium as a nuclear fuel. They include:

the high cost of fuel fabrication, due partly to the high radioactivity of 233U, which is a result of its contamination with traces of the short-lived 232U;
similar difficulties in recycling thorium, due to highly radioactive 228Th;
some weapons proliferation risk of 233U.
Thus, much development work is required before the thorium fuel cycle can be commercialized.
Nevertheless, the thorium fuel cycle, with its potential for breeding fuel without the need for fast neutron reactors, holds considerable potential for the long term. Thorium is significantly more abundant than uranium, so it is a key factor in the sustainability of nuclear energy.
India, which has about 25 percent of the world's total reserves,[1] has planned its nuclear power program to eventually use thorium exclusively, phasing out uranium as an input material. This ambitious plan uses both fast and thermal breeder reactors. The Advanced Heavy Water Reactor and KAMINI reactor are efforts in this direction.

Precautions
Powdered thorium metal is often pyrophoric and should be handled with care. Moreover, exposure to aerosolized thorium can lead to increased risk of cancers of the lung, pancreas, and blood. Exposure to thorium internally leads to increased risk of liver diseases. This element has no known biological role.

See also
Chemical element
Inner transition metal
Periodic table
Radioactive decay
Footnotes

↑ 1.0 1.1 US approves Indian nuclear deal. BBC News (December 9, 2006). Retrieved December 17, 2007.

↑ Information and Issue Briefs - Thorium. World Nuclear Association. Retrieved June 1, 2006. Retrieved December 16, 2007.

↑ van Arkel, A.E. and de Boer, J.H. (1925).  Preparation of pure titanium, zirconium, hafnium, and thorium metal. Zeitschrift für Anorganische und Allgemeine Chemie 148: 345-350.

↑ Phys. Rev. C 52, 113–116 (1995)


ReferencesISBN links support NWE through referral fees
Chang, Raymond. 2006. Chemistry, ninth ed. New York: McGraw-Hill Science/Engineering/Math. ISBN 0073221031
Cotton, F. Albert and Geoffrey Wilkinson. 1980. Advanced Inorganic Chemistry, 4th ed. New York: Wiley. ISBN 0-471-02775-8
Greenwood, N.N. and A. Earnshaw. 1998. Chemistry of the Elements, 2nd Edition. Oxford, U.K.; Burlington, Massachusetts: Butterworth-Heinemann, Elsevier Science. ISBN 0750633654
Thorium WebElements.com. Retrieved December 17, 2007.
Thorium Los Alamos National Laboratory. Retrieved December 17, 2007.
The Uranium Information Centre provided some of the original material in this article. Retrieved December 17, 2007.
van Arkel, A.E., and de Boer, J.H. 1925. Preparation of pure titanium, zirconium, hafnium, and thorium metal: Zeitschrift für Anorganische und Allgemeine Chemie, v. 148, p. 345-350.
External links
All links retrieved March 12, 2020.

Thorium USGS data.

Credits
New World Encyclopedia writers and editors rewrote and completed the Wikipedia article
in accordance with New World Encyclopedia standards. This article abides by terms of the Creative Commons CC-by-sa 3.0 License (CC-by-sa), which may be used and disseminated with proper attribution. Credit is due under the terms of this license that can reference both the New World Encyclopedia contributors and the selfless volunteer contributors of the Wikimedia Foundation. To cite this article click here for a list of acceptable citing formats.The history of earlier contributions by wikipedians is accessible to researchers here:

Thorium  history
The history of this article since it was imported to New World Encyclopedia:

History of "Thorium"
Note: Some restrictions may apply to use of individual images which are separately licensed.